REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS


 Terence Joseph
 1 years ago
 Views:
Transcription
1 20 th International Conference on Composite Materials Copenhagen, th July 2015 REPRESENTING MATRIX CRACKS THROUGH DECOMPOSITION OF THE DEFORMATION GRADIENT TENSOR IN CONTINUUM DAMAGE MECHANICS METHODS Frank A. Leone, Jr. 1 1 Structural Mechanics and Concepts Branch, NASA Langley Research Center Hampton, VA, USA web page: Keywords: Continuum damage mechanics; progressive damage analysis; finite element method This paper is the work of the U.S. Government and is not subject to copyright protection in the U.S. ABSTRACT A method is presented to represent the largedeformation kinematics of intraply matrix cracks and delaminations in continuum damage mechanics (CDM) constitutive material models. The method involves the additive decomposition of the deformation gradient tensor into crack and bulk material components. The response of the intact bulk material is represented by a reduced deformation gradient tensor, and the opening of an embedded cohesive interface is represented by a normalized cohesive displacementjump vector. The rotation of the embedded interface is tracked as the material deforms and as the crack opens. The distribution of the total local deformation between the bulk material and the cohesive interface components is determined by minimizing the difference between the cohesive stress and the bulk material stress projected onto the cohesive interface. The improvements to the accuracy of CDM models that incorporate the presented method over existing approaches are demonstrated for a single element subjected to simple shear deformation and for a finite element model of a unidirectional openhole tension specimen. The material model is implemented as a VUMAT user subroutine for the Abaqus/Explicit finite element software. The presented deformation gradient decomposition method reduces the artificial load transfer across matrix cracks subjected to large shearing deformations, and avoids the spurious secondary failure modes that often occur in analyses based on conventional progressive damage models. 1 INTRODUCTION The National Aeronautics and Space Administration (NASA) Advanced Composites Project (ACP) has the goal to reduce current 5 10 year product development and certification timelines by 30 percent for composite material aerospace applications. The first technical challenge of ACP involves the assessment and improvement of computational tools capable of predicting the strength and life of composite aerospace structures. A wide range of computational tools exist for the modeling of progressive damage in composite materials, including cohesive zone modeling, continuum damage mechanics, peridynamics, the extended finite element method, etc. In continuum damage mechanics (CDM) models, the presence of a crack is accounted for by modifying select terms of the material stiffness tensor C. The terms of the damaged material stiffness tensor C d are set so that the stress σ calculated from the current strain ε accounts for the opening of the crack without explicitly modeling the crack itself (i.e., without changing the original mesh or introducing additional degrees of freedom to the model): σ = C d : ε (1) The terms of the material stiffness tensor that are modified are often selected based on the assumption that crack normals are aligned with the principal material directions, e.g., softening the fiberdirection Young s modulus for fiber failure, or softening the matrixdirection Young s modulus and shear modulus for matrix failure. Several such plylevel, strainbased CDM models have been developed for
2 Frank A. Leone, Jr. fiberreinforced materials with varying degrees of sophistication (e.g., [1 4]) and the models generally perform well for representing the formation and development of damage, especially when applied in cases where the loading is primarily planar and failure is quasibrittle. Camanho et al. [5] developed a threedimensional CDM material model that embeds a cohesive interface in a continuum to represent a matrix crack. The use of a cohesive interface to represent matrix damage allows for consistent intraply and interply mixedmode matrix damage predictions and better represents the kinematics of a softened interface that is not necessarily aligned with the principal material directions. The orientation of the cohesive interface within the material is defined based on the predictions of a threedimensional matrix failure criterion. Camanho s model is a smearedcrack approach that utilizes additive strain decomposition to separate the strain tensor supplied by the finite element (FE) solver into linear elastic and cracking strain components: ε = ε el + ε cr (2) where ε el represents the linear elastic deformation of the bulk material and ε cr represents the embedded cohesive displacementjump. The distribution between the elastic and cracking strain components is determined by solving for the cohesive displacementjump vector that minimizes the difference between the cohesive stress vector and the bulk material stress tensor projected onto the cohesive interface. The Camanho model is implemented as a VUMAT user material subroutine for use with threedimensional solid elements in Abaqus/Explicit [6]. Model results were shown to correlate well with experimental loaddisplacement results for unidirectional offaxis compression, laminated centercracked tension, and laminated openhole tension specimens. However, CDM material models based on strain measures can suffer from difficulties regarding the definition of the orientation of a crack with respect to the orientation of a continuum for problems involving large shear deformation. In geometrically nonlinear models, elements are formulated in the current configuration using current nodal positions, and the strain ε is derived from the current configuration of the material [6]. The use of the FE solversupplied strain as the input to CDM material models in geometrically nonlinear models can cause the current crack orientation to be erroneously defined, with the magnitude of the error scaling up with shear deformation. For example, consider a twodimensional continuum that contains a crack with a normal in the reference 2direction. When subjected to simple shear deformation, the orientation of the continuum rotates. If the orientation of an open crack is defined in terms of the FE solversupplied strain in the current configuration, the orientation of the crack normal also rotates. For a cracked continuum subjected to simple shear, however, the orientations of the bulk material and the crack should not rotate. An incorrectly defined matrix crack orientation can cause load transfer across matrix cracks and the prediction of spurious secondary failure mechanisms (e.g., fiber failure). In order to address these issues, CDM material models must better account for the kinematics of a cracked continuum. Similar to the smearedcrack CDM material model of Camanho et al. [5], the continuumdecohesive finite element (CDFE) of Prabhakar and Waas [7] utilizes an embedded cohesive law to represent the formation and growth of intraply cracks in fiberreinforced materials. The CDFE method is a finite element formulation that involves applying the principle of virtual work to a cracked continuum, deriving an enriched set of displacements for real and internal dummy nodes, and generating an equivalent element stiffness for the cracked element through static condensation. The CDFE method has been implemented as a twodimensional triangular element for use with an inhouse code at the University of Michigan. Results of openhole tension specimen models with various fiber orientations were solved, yielding good correlation with experimental strain and displacement fields measured by digital image correlation. Finite element techniques that are specially developed for modeling cracks within solid materials, such as the extended finite element method (e.g., [8 10]) and the CDFE method [7], do not exhibit the geometrically nonlinear crack orientation issues of conventional strainbased CDM methods. However, the implementation of these specialized finite elements in commercial finite element solvers can be
3 20 th International Conference on Composite Materials Copenhagen, th July 2015 difficult and precludes the use of existing finite element libraries. To take advantage of all of the existing builtin capabilities of commercial FE programs, it is desirable to use constitutive material models to model damage, while achieving a predictive capability similar to those of specialized finite elements. This paper presents an improved approach for representing the kinematics of the formation, opening, and closure of matrix cracks in CDM material models for fiberreinforced materials. The method, which was originally outlined in reference [11] and presented in detail in reference [12], is an extension of the smearedcrack CDM material model of Camanho et al. [5] with improved predictive capability for geometrically nonlinear problems, especially when subject to large shear deformations. Section 2 of this paper presents the details of the deformation gradient decomposition (DGD) method. Section 3 presents FE model results for two case studies and compares results generated with a conventional strainbased CDM material model and with a CDM material model based on the DGD method. 2 DEFORMATION GRADIENT DECOMPOSITION CDM METHOD The DGD method is based on the additive decomposition of the deformation gradient tensor F, analogous to the additive strain decomposition of the smearedcrack model defined by equation (2). The two decomposed components of F are (i) the deformation gradient tensor F B, which represents the bulk material deformation, and (ii) the cohesive displacementjump vector δ, which represents the deformation of an embedded cohesive crack. The derivation of the DGD method is carried out at the constitutive material level so as to be compatible with any commercial finite element code with userdefined material subroutines. The DGD method is herein presented in the context of being implemented as a VUMAT user material subroutine for use with threedimensional solid elements in Abaqus/Explicit, although the general concepts are applicable to conventional and continuum shell elements as well. In section 2.1, the coordinate systems for the continuum, the bulk material, and the embedded cohesive crack are defined in the reference and current configurations. In section 2.2, the decomposition of the deformation gradient tensor is performed so as to provide consistent definitions for the bulk material and cohesive crack deformations. In section 2.3, local equilibrium is established between the bulk material and cohesive crack components, which allows the bulk material strain and stress to be calculated and the cohesive damage variable to be determined. 2.1 Bulk Material and Crack Coordinate Systems A rectangular cuboidal continuum of fiberreinforced material with the fiber direction initially aligned with the reference x 1 direction is considered. The undeformed continuum may contain a matrix crack with a crack normal e N oriented at an angle α from the x 2 direction in the x 2 x 3 plane, as shown in Figure 1. The angle α is defined in the reference configuration and does not change once determined. The angle α is dependent on the local stress state and can be determined by using a failure criterion for fiberreinforced materials that accounts for the stress state on the angle of the fracture plane (e.g., [13, 14]). For the present method, α may take on values from tan 1 (l 2 l 3 ) to π tan 1 (l 2 l 3 ). The initial, undeformed reference configuration of the continuum is described by X R. The three columns of X R are orthogonal vectors designated X R (1), XR (2), and XR (3), with lengths equal to the undeformed dimensions of the continuum, l 1, l 2, and l 3, respectively, such that: l X R = [ 0 l 2 0 ] (3) 0 0 l 3 The current configuration of the continuum, x, is a function of X R and the deformation gradient tensor F: x = FX R (4)
4 Frank A. Leone, Jr. x 3 x 2 x 1 Figure 1: Schematic showing the orientation of the crack and dimensions of the continuum in the reference configuration. [12] The deformation gradient tensor F maps the coordinates defined in the reference configuration to their relative locations in the current configuration. F is easily computed from nodal displacements and is a known quantity that is generally provided by FE solvers as an input for userdefined material models. The reference configurations of the bulk material and the continuum are equal, as it is assumed that there is no crack exists while initially undeformed. The current configuration of the bulk material, x B, is a function of X R and bulk material deformation gradient tensor F B : x B = F B X R (5) Prior to the initiation of damage, F B and F are equal. The method for solving for F B after the initiation of damage is presented in sections 2.2 and 2.3. The orientation of the crack within the continuum can be described in terms of orthogonal unit vectors in the fiber, cracknormal, and transverse directions, e F, e N, and e T, respectively, as shown in Figure 1. These three unit vectors form the basis of the coordinate system R cr : R cr = [e F e N e T] (6) In the reference configuration, the basis vectors of R cr depend only on α. In the current configuration, however, the deformation of the bulk material must be considered. For cases in which the crack is open, R cr is a function of F B and α: 1 e F = F B [ 0] (7a) 0 0 T e N = F B [ cos α] (7b) sin α e T = e F e N where e F, e N, and e T are the nonnormalized basis vectors of R cr. 2.2 Decomposition of the Deformation Gradient Tensor The bulk material deformation gradient tensor F B can be derived as a function of F and δ. Once a converged solution for F B is found, the stress and strain of the bulk material can be defined for any arbitrary deformation and any arbitrary angle α. (7c)
5 20 th International Conference on Composite Materials Copenhagen, th July 2015 A schematic relationship is shown in Figure 2 between the deformation of the continuum (x) and the deformations of its bulk material (x B ) and cohesive crack (δ) components in the x 1 x 2 plane for α = 0. In the figure, the crack is shown as being located along the top surface of the continuum, for clarity. However, the exact location of the crack within the continuum is ambiguous in CDM methods. As a result, it is necessary to make an assumption regarding the path of the crack through the continuum. In the present model, it is assumed that the crack crosses the continuum so as to intersect opposite pairs of surfaces of the continuum, i.e., the crack plane always intersects the surfaces whose normals are aligned with the x 1 direction in the reference configuration, and it intersects the surfaces whose normals are aligned with either the x 2  or x 3 directions in the reference configuration., Figure 2: Decomposition of x 2 direction deformation for a partially opened crack with a crack normal e N oriented at α = 0. The first column of F B can be obtained from F by considering that the fiberdirection deformation does not depend on the presence, opening, or orientation of any matrix cracks. Because the cracknormal direction is always normal to the fiberdirection, the current configurations of X R (1) calculated using F and F B, x (1) and x B (1), respectively, are always equal: x (1) = x B (1) FX R (1) = FB X R (1) (8a) (8b) Because only the first component of X R (1) is nonzero, equation (8b) yields: F B (1) = F (1) (8c) where F (1) is the first column of F and F B (1) is the first column of F B. For the crack shown in Figure 2, X R (2) is intersected by the crack plane. As a result, the current configuration x (2) is equal to the vector sum of the bulk material response x B (2) and the cohesive displacementjump vector δ transformed into the reference configuration: x (2) = x B (2) + Rcr δ FX R (2) = FB X R (2) + Rcr δ (9a) (9b) Because only the second component of X R (2) is nonzero, equation (9b) yields:
6 Frank A. Leone, Jr. F B (2) = F (2) 1 l 2 R cr δ (9c) where F (2) is the second column of F and F B (2) is the second column of F B. For the crack shown in Figure 2, X R (3) is not intersected by the crack. As a result, FB (3) can be derived using logic similar to the derivation of F B (1), yielding: F B (3) = F (3) (10) where F (3) is the third column of F and F B (3) is the third column of F B. For cases in which the crack intersects X R (3) instead of XR (2), the derivations for the second and third columns of FB are swapped. In order to write a generalized equation for F B, it is necessary to account for whether the crack plane intersects X R (2) or XR (3), which depends on α, l2, and l 3. The integer q can be used to define whether the (2) (3) crack intersects X R or XR. When α tan 1 (2) (l 2 l 3 ), the crack plane intersects X R and q = 2. When α > tan 1 (3) (l 2 l 3 ), the cohesive crack intersects X R and q = 3. A generalized equation for the deformation gradient tensor decomposition can then be written: F (q) l q = F B (q) l q + R cr δ (11) where F (q) is the qth column of F, F B (q) is the qth column of F B, and l q is the length of the qth column of X R. Using equation (11) with any F provided by the finite element solver, the cohesive displacementjump vector δ can be solved for in terms of F B (q). 2.3 Equilibrium between the Bulk Material and Cohesive Crack The sum of the bulk material deformation and the cohesive displacementjump is shown in equation (11) to be equal to the deformation described by the deformation gradient tensor. However, it remains necessary to ensure that the tractions resulting from the deformations of the bulk material and cohesive crack are in equilibrium. In the present method, equilibrium is enforced on the cohesive crack plane with the normal e N. The solution for the current bulk deformation gradient is found by minimizing the difference between the cohesive stress vector τ and the bulk material stress σ B projected onto the cohesive crack. The cohesive stress vector τ is determined using the cohesive damage model of González et al. [15] is used. The cohesive stress vector τ is defined as: k F (1 d m )δ F τ = [ k N (1 d m )δ N k N d m δ N ] (12) k T (1 d m )δ T where δ N is the opening displacementjump, and δ F and δ T are the shear displacementjumps along the fiber and transverse directions, respectively; k F, k N, and k T are the cohesive penalty stiffnesses in the fiber, cracknormal, and transverse directions, respectively; d m is the scalar cohesive damage variable; and the operator x is defined as x = (x + x ) 2. The bulk material stress is determined from the bulk material deformation gradient tensor F B using standard finite stress and strain definitions and Hooke s Law: T E = (F B F B I) 2 (13) S = C d : E (14) where E is the GreenLagrange strain, S is the 2 nd PiolaKirchhoff stress, and I is the identity tensor. Tensile fiber failure initiation is predicted using an uncoupled maximum strain failure criterion with the
7 20 th International Conference on Composite Materials Copenhagen, th July 2015 fiberdirection GreenLagrange strain. Fiber damage is represented using the CDM approach of Maimí et al. [2]. Cauchy s stress theorem is used to find the corresponding stress vector t acting on the cohesive interface: t = σ B e N (15) where σ B is the bulk material Cauchy stress in the reference coordinate system, determined using: σ B = F B S F B T F B 1 (16) To solve for the stress state at equilibrium, a residual stress vector σ Res can be defined in terms of the components of the stress vectors in equations (12) and (15) in the current crack coordinate system: k F (1 d m )δ F t e F σ Res = [ k N (1 d m )δ N k N d m δ N t e N ] (17) k T (1 d m )δ T t e T Because F is known and δ is a function of F and F B, the three components of F B (q) are used as the unknown variables that must be found in order to minimize the residual. The multivariate Newton Raphson method is used to find a converged solution for F B (q) : 1 F (q) B,new = F (q) B ( σ Res F (q)) B σ Res (18) A solution is sought until the norm of σ Res is less than a userdefined tolerance value, set by default to 0.01% of the mode I cohesive strength. After a converged solution is found, the cohesive damage model is evaluated for the current δ. If the cohesive damage variable d m is predicted to increase, a new converged deformation state is sought for the updated d m using equation (18). If d m is not predicted to increase, a solution for the current material state has been found, and the results are reported to the FE solver. 3 CASE STUDIES Two case studies demonstrating the predictive capability of the DGD method for geometrically nonlinear problems involving large shear deformations are presented. The first case study is a single element subjected to simple shear deformation. The second case study is a unidirectional openhole tension (OHT) specimen based on a previous experimental and analytical investigation by Iarve et al. [16]. For each example, FE models were developed and solved using Abaqus/Explicit under quasistatic loading conditions with geometric nonlinearity considered [6]. To demonstrate the advantages of incorporating DGD into current CDM modeling approaches, the two case study models were solved using: (i) the presented DGD CDM method, and (ii) an implementation of the smearedcrack model of Camanho et al. [5] to represent the predictions of a strainbased CDM method. Additional strainbased CDM methods were evaluated, and similar results were found for all strainbased CDM methods evaluated for the two case study models. Predictions obtained using the two material models are evaluated and compared in terms of how the local stresses are affected by predicted matrix cracks and in terms of the details of the predicted overall failure processes. 3.1 Single Element Simple Shear A single threedimensional element is deformed in simple shear in the x 1 x 2 plane. The element measures 0.1 mm on each side and is composed of IM7/8552 carbon/epoxy material. The 0 fiber direction is aligned with the x 1 direction. The relevant material properties for IM7/8552 are provided in Table 1. An eightnode C3D8R solid element with reduced integration is used. The four nodes on the surface at x 2 = 0 mm are constrained in the x 1  and x 2 directions. The four nodes on the surface at x 2 = 0.1 mm are constrained in the x 2 direction and displaced 0.05 mm in the positive x 1 direction. The four nodes on the surface at x 3 = 0 mm are constrained in the x 3 direction.
8 Shear Stress [MPa] Frank A. Leone, Jr. Property Description Value Ref. E 1 Young s modulus, fiberdirection 171,420 MPa [17] E 2 Young s modulus, matrixdirection 9,080 MPa [17] G 12 Shear modulus 5,290 MPa [17] ν 12 Poisson ratio, [17] ν 23 Poisson ratio, [5] Y T Mode I matrix strength 62.3 MPa [17] S L Mode II matrix strength 92.3 MPa [17] X ft Fiber tensile strength 2,326 MPa [17] G Ic Mode I matrix fracture toughness kj/m 2 [17] G IIc Mode II matrix fracture toughness kj/m 2 [17] η BenzeggaghKenane coefficient [5] G ft Fiber tensile fracture toughness 134. kj/m 2 [18] Table 1: IM7/8552 material properties. The expected response to simple shear deformation is an initially linearelastic response leading up to the formation of a matrix crack (i.e., d m > 0) with a crack normal in the x 2 direction, followed by mode II dominant linear softening until the crack is fully formed (i.e., d m = 1). After d m = 1, all stress components should be equal to zero, as any further simple shear deformation should then represent the sliding of two separated, undeformed volumes of material. The model using the DGD CDM method predicts a nearly perfect mode II response to simple shear deformation, as is evident by the shear stressdisplacement results shown in Figure 3. Even at large shear displacements, no load transfer across the crack is observed. The model with the strainbased CDM method accurately predicts the initiation of matrix damage and the initial rate of energy dissipation, as expected. With increasingly large shear deformation, however, increasingly large load transfer across the matrix crack is observed Strainbased CDM DGDbased CDM Shear Displacement [mm] Figure 3: Shear stressdisplacement FE results for the single element simple shear model. Shear stress is calculated as the sum of the x 1 direction nodal forces of the nodes on the +x 2 direction surface of the element, divided by 0.01 mm 2. [12] The use of incorrectly defined coordinate systems for the crack and the bulk material can also lead to the prediction of spurious, secondary failure modes. For instance, the simple shear model with the strainbased CDM method predicts increasing compressive fiber stresses with increasing simple shear deformation after the formation of the matrix crack. With increasing shear deformation, these
9 20 th International Conference on Composite Materials Copenhagen, th July 2015 nonphysical compressive fiber stresses in the model with the strainbased CDM method eventually satisfy the compressive fiber failure criterion, causing spurious fiber damage initiation (not shown in Figure 3). 3.2 Unidirectional OpenHole Tension A model of a unidirectional [0 8] openhole tension specimen is shown in Figure 4. The specimen has a length l equal to 50.8 mm, a width w equal to 12.7 mm, and a thickness t equal to 1.0 mm. The specimen contains a hole at its center with a diameter d equal to mm. The fiberdirection is aligned with the specimen length. The nodes on the surface at x 1 = 0 are constrained in the x 1 direction. The nodes along the edge at x 1 = 0 and x 2 = 0 and the edge at x 1 = l and x 2 = 0 are constrained in the x 2  direction. The nodes on the surfaces at x 1 = 0 and x 1 = l are constrained in the x 3 direction. Load is introduced by uniformly displacing the nodes on the surface at x 1 = l in the positive x 1 direction. Threedimensional, eightnode C3D8R solid elements with reduced integration are used. The mesh lines are aligned with the fiber direction to avoid shear stress transfer due to element shear locking, based on the recommendations of Song et al. [19] for similar laminated OHT models. All of the elements along the expected matrix splitting path are cuboids and have an element length equal to mm in the x 2 direction. Four layers of elements of equal thickness are used through the thickness of the laminate. Figure 4: Mesh and geometry for the unidirectional OHT FE model. [12] Based on the experimental work of Iarve et al. presented in reference [15], the expected failure process for the unidirectional OHT specimen is as follows: (i) matrix splitting cracks form tangent to the hole and extend along the x 1 direction toward the model edges; (ii) as the matrix cracks extend, the fiber stress concentration at the hole diminishes until a uniform σ 11 stress state is established in the remaining ligaments on either side of the hole; (iii) the specimen fails when σ 11 in the ligaments reaches X ft at a load of approximately: 22.2 kn = X ft (w d) t (19) Because no compressive matrix or fiber damage should occur in the model, and to better isolate the effects of defining the material stress state via the DGD method, the compressive matrix and fiber strength and fracture toughness properties for the strainbased CDM model were artificially increased to avoid their activation in this study. Analysis predictions obtained with the model using the DGD CDM model are represented by the black curve in Figure 5, and the predictions match the expected failure process [15]. Matrix damage initiation occurs at four locations that are tangent to the hole at an applied tensile load of 2.4 kn. At a tensile load of 4.2 kn, the four matrix splitting cracks rapidly extend along the length of the specimen to an average length of 17 mm. Cracks of this length reduce the stiffness of the specimen, as can be seen in Figure 5 with a shift in the curve. The matrix splitting cracks then propagate slowly toward the model edges with continued loading. A peak load of 22.3 kn is reached just prior to tensile fiber failure
10 Load [kn] Frank A. Leone, Jr. originating at the edge of the hole in the intact ligaments. The extent of predicted matrix damage is shown by the red elements just prior to failure in Figure 6a. The OHT model with the strainbased CDM model predicts matrix crack initiation and the initial growth of the matrix cracks at loads in close agreement with the DGD model predictions. However, when the cracked elements undergo large shear deformation, load transfer across the cracked elements occurs and further matrix crack growth is slowed. The slower rate of matrix splitting crack growth predicted by the strainbased CDM model is apparent in the slower rate of change in the slope of the loaddisplacement response, as shown by the gray curve in Figure 5. Load transfer across the first set of four matrix splitting cracks causes secondary and tertiary rows of matrix cracks to develop, as shown in in Figure 6b. Regions of the mesh where multiple adjacent matrix cracks develop (i.e., rows of softened elements without any intact elements remaining between them) undergo severe distortion. The distortion of the mesh leads to premature failure of the model at a load of 9.6 kn Strainbased CDM DGD CDM Failure caused by mesh distortion Matrix splitting cracks fully develop Displacement [mm] Figure 5: Loaddisplacement results of the unidirectional OHT models. [12] (a) DGD CDM method Excessive mesh distortion Secondary and tertiary row s of parallel matrix spitting cracks (b) Strainbased CDM method Figure 6: Predicted matrix damage state at peak load for the unidirectional OHT models. Blue represents intact material and red represents a fully developed matrix crack. [12]
11 Normalized Stress Normalized Stress 20 th International Conference on Composite Materials Copenhagen, th July 2015 Iarve et al. [15] and Song et al. [19] demonstrated that CDM methods are unable to eliminate the stress concentration at the hole that should follow the formation of the splitting cracks, and the present results confirm those observations. Stress concentration factors equal to approximately 1.5 are predicted by the model with the strainbased CDM method after the formation of the matrix splitting cracks, as shown in Figure 7a. The analysis conducted with the DGD CDM method predicts a more uniform σ 11 distribution after the extension of the matrix splitting cracks, as shown in Figure 7b kn kn kn kn kn 8 kn kn 8 kn Normalized Distance (a) Strainbased CDM method Normalized Distance (b) DGD CDM method Figure 7: Normalized fiberdirection stress versus normalized distance from the hole along the midsection of the unidirectional OHT model. The fiberdirection stress is normalized by E 1 Δ L, where Δ is the applied x 1 direction displacement and L is the specimen length. 4 CONCLUSIONS The deformation gradient decomposition (DGD) method improves the predictive capability of continuum damage mechanics (CDM) methods for fiberreinforced materials in geometrically nonlinear finite element models. The DGD method involves the additive decomposition of the deformation gradient tensor into crack and bulk material components and determines the current crack opening displacement by assuming stress equivalence on the crack plane. The DGD method accurately represents crack kinematics in CDM progressive damage analyses. The implementation of the DGD method within a constitutive material model allows for the method to be applied to existing two or threedimensional solid or shell finite elements. The potential improvements to the accuracy of progressive damage finite element models have been demonstrated for a single element subjected to simple shear deformation and for a tensionloaded unidirectional openhole specimen model. In both cases, the DGD method performs better than existing strainbased approaches in terms of reducing the transfer of load across open matrix cracks and avoiding the prediction of spurious secondary failure modes when subjected to large shear deformations. REFERENCES [1] Matzenmiller A, Lubliner J, Tayler RL. A constitutive model for anisotropic damage in fibercomposites. Mechanics of Materials 1995; 20: [2] Maimí P, Camanho PP, Mayugo JA, Dávila CG. A continuum damage model for composite laminates: Part I Constitutive model. Mechanics of Materials 2007; 39: [3] Lapcyzyk I, Hurtado JA. Progressive damage modeling in fiberreinforced materials. Composites Part A: Applied Science and Manufacturing 2007; 38:
12 Frank A. Leone, Jr. [4] Van Der Meer FP, Sluys LJ. Continuum models for the analysis of progressive failure in composite laminates. Journal of Composite Materials 2009; 43(20): [5] Camanho PP, Bessa MA, Catalanotti G, Vogler M, Rolfes R. Modeling the inelastic deformation and fracture of polymer composites Part II: Smeared crack model. Mechanics of Materials 2013; 59: [6] ABAQUS (2013). Abaqus 6.13 Online Documentation. Dassault Systèmes, Providence, RI, USA. [7] Prabhakar P, Waas AM. A novel continuumdecohesive finite element for modeling inplane fracture in fiber reinforced composites. Composites Science and Technology 2013; 83:1 10. [8] Ling D, Yang Q, Cox B. An augmented finite element method for modeling arbitrary discontinuities in composite materials. International Journal of Fracture 2009; 156: [9] Iarve EV, Gurvich MR, Mollenhauer DH, Rose CA, Dávila CG. Meshindependent matrix cracking and delamination modeling in laminated composites. International Journal for Numerical Methods in Engineering 2011; 88(8): [10] Chen BY, Pinho ST, De Carvalho NV, Baiz PM, Tay TE. A floating node method for the modeling of discontinuities in composites. Engineering Fracture Mechanics 2014; 127: [11] Rose CA, Dávila CG, Leone FA. Analysis methods for progressive damage of composite structures. NASA/TM [12] Leone FA. Deformation gradient tensor decomposition for representing matrix cracks in fiberreinforced materials. Composites Part A: Applied Science and Manufacturing (submitted). [13] Pinho ST, Dávila CG, Camanho PP, Iannucci L, Robinson P. Failure models and criteria for FRP under inplane or threedimensional stress states including shear nonlinearity. NASA/TM [14] Catalanotti G, Camanho PP, Marques AT. Threedimensional failure criteria for fiberreinforced laminates. Composite Structures 2013; 95: [15] González EV, Maimí P, Turon A, Camanho PP, Renart J. Simulation of delamination by means of cohesive elements using an explicit finite element code. Computers, Materials and Continua 2009; 9(1): [16] Iarve EV, Mollenhauer D, Kim R. Theoretical and experimental investigation of stress redistribution in open hole composite laminates due to damage accumulation. Composites Part A: Applied Science and Manufacturing 2005; 36(2): [17] Camanho PP, Maimí P, Dávila CG. Prediction of size effects in notched laminates using continuum damage mechanics. Composites Science and Technology 2007; 67: [18] Catalanotti G, Camanho PP, Xavier J, Dávila CG, Marques AT. Measurement of resistance curves in the longitudinal failure of composites using digital image correlation. Composites Science and Technology 2010; 70: [19] Song K, Li Y, Rose CA. Continuum damage mechanics models for the analysis of progressive failure in openhole tension laminates. 52nd AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics and Materials Conference. 4 7 April Denver, Colorado.
FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FLOATING NODE METHOD AND VIRTUAL CRACK CLOSURE TECHNIQUE FOR MODELING MATRIX CRACKING DELAMINATION MIGRATION N. V. De Carvalho 1*, B. Y. Chen
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationNumerical simulation of delamination onset and growth in laminated composites
Numerical simulation of delamination onset and growth in laminated composites G. Wimmer, C. Schuecker, H.E. Pettermann Austrian Aeronautics Research (AAR) / Network for Materials and Engineering at the
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More information6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS
6. NONLINEAR PSEUDOSTATIC ANALYSIS OF ADOBE WALLS Blondet et al. [25] carried out a cyclic test on an adobe wall to reproduce its seismic response and damage pattern under inplane loads. The displacement
More informationUniversity of Bristol  Explore Bristol Research. Early version, also known as preprint
Hallett, S. R., & Wisnom, M. R. (2006). Numerical investigation of progressive damage and the effect of layup in notched tensile tests. Journal of Composite Materials, 40 (14), 12291245. DOI: 10.1177/0021998305057432
More informationQUESTION BANK Composite Materials
QUESTION BANK Composite Materials 1. Define composite material. 2. What is the need for composite material? 3. Mention important characterits of composite material 4. Give examples for fiber material 5.
More informationComposite Materials 261 and 262
Composite Materials 261 and 262 Stefan Hartmann 1 David Moncayo 2 1 DYNAmore GmbH, Stuttgart, Germany 2 Daimler AG, Sindelfingen, Germany 11. LSDYNA Forum 2012, 9.  10. Oktober 2012, Ulm 1 Outline Introduction
More informationPrediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads
Prediction of Delamination Growth Behavior in a Carbon Fiber Composite Laminate Subjected to Constant Amplitude CompressionCompression Fatigue Loads J. Raju 1*, D.S. Sreedhar 2, & C.M. Manjunatha 1 1
More informationISSN: ISO 9001:2008 Certified International Journal of Engineering Science and Innovative Technology (IJESIT) Volume 2, Issue 4, July 2013
Delamination Studies in FibreReinforced Polymer Composites K.Kantha Rao, Dr P. Shailesh, K. Vijay Kumar 1 Associate Professor, Narasimha Reddy Engineering College Hyderabad. 2 Professor, St. Peter s Engineering
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationFASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FASTENER PULLTHROUGH FAILURE IN GFRP LAMINATES G. Catalanotti 1*, P.P. Camanho 1, P. Ghys 2, A.T. Marques 1 1 DEMec, Faculdade de Engenharia, Universidade
More informationDAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS DAMAGE SIMULATION OF CFRP LAMINATES UNDER HIGH VELOCITY PROJECTILE IMPACT A. Yoshimura 1*, T. Okabe, M. Yamada 3, T. Ogasawara 1, Y. Tanabe 3 1 Advanced
More informationLectures on. Constitutive Modelling of Arteries. Ray Ogden
Lectures on Constitutive Modelling of Arteries Ray Ogden University of Aberdeen Xi an Jiaotong University April 2011 Overview of the Ingredients of Continuum Mechanics needed in Soft Tissue Biomechanics
More informationMultiscale Approach to Damage Analysis of Laminated Composite Structures
Multiscale Approach to Damage Analysis of Laminated Composite Structures D. Ivančević and I. Smojver Department of Aeronautical Engineering, Faculty of Mechanical Engineering and Naval Architecture, University
More informationCrash and Impact Simulation of Composite Structures by Using CAE Process Chain
Crash and Impact Simulation of Composite Structures by Using CAE Process Chain Madhukar Chatiri 1, Thorsten Schütz 2, Anton Matzenmiller 3, Ulrich Stelzmann 1 1 CADFEM GmbH, Grafing/Munich, Germany, mchatiri@cadfem.de
More informationFinite ElementBased Failure Models for Carbon/Epoxy Tape Composites
Finite ElementBased Failure Models for Carbon/Epoxy Tape Composites A Master Thesis Presented to The Academic Faculty by Guillaume Seon In Partial Fulfillment of the Requirements for the Degree Master
More informationCrashworthy Design of Composite Structures Using CAE Process Chain
0 th European LSDYNA Conference 205, Würzburg, Germany Crashworthy Design of Composite Structures Using CAE Process Chain Madhukar Chatiri, Thorsten Schuetz 2, Anton Matzenmiller 3 CADFEM GmbH, Grafing
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More informationA FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
TRENDS IN COMPUTATIONAL STRUCTURAL MECHANICS W.A. Wall, K.U. Bletzinger and K. Schweizerhof (Eds.) c CIMNE, Barcelona, Spain 2001 A FINITE ELEMENT MODEL FOR THE ANALYSIS OF DELAMINATIONS IN FRP SHELLS
More informationDynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models
Dynamic Analysis of a Reinforced Concrete Structure Using Plasticity and Interface Damage Models I. Rhee, K.J. Willam, B.P. Shing, University of Colorado at Boulder ABSTRACT: This paper examines the global
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More information3D Finite Element analysis of stud anchors with large head and embedment depth
3D Finite Element analysis of stud anchors with large head and embedment depth G. Periškić, J. Ožbolt & R. Eligehausen Institute for Construction Materials, University of Stuttgart, Stuttgart, Germany
More informationGeneric Strategies to Implement Material Grading in Finite Element Methods for Isotropic and Anisotropic Materials
University of Nebraska  Lincoln DigitalCommons@University of Nebraska  Lincoln Engineering Mechanics Dissertations & Theses Mechanical & Materials Engineering, Department of Winter 1292011 Generic
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationTHE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH
THE ROLE OF DELAMINATION IN NOTCHED AND UNNOTCHED TENSILE STRENGTH M. R. Wisnom University of Bristol Advanced Composites Centre for Innovation and Science University Walk, Bristol BS8 1TR, UK M.Wisnom@bristol.ac.uk
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More informationBUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION
2 th International Conference on Composite Materials Copenhagen, 1924 th July 215 BUCKLING AND POSTBUCKLING IN FILAMENT WOUND COMPOSITE TUBES UNDER TRANSVERSE COMPRESSION José Humberto S. Almeida Jr.
More informationModeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress
Modeling Hailstone Impact onto Composite Material Panel Under a Multiaxial State of Stress Authors Marco ANGHILERI * LuigiM L CASTELLETTI * Andrea MILANESE * and Andrea SEMBOLONI * Affiliation * Politecnico
More informationInfluence of the filament winding process variables on the mechanical behavior of a composite pressure vessel
Influence of the filament winding process variables on the mechanical behavior of a composite pressure vessel G. Vargas 1 & A. Miravete 2 1 Universidad Pontificia Bolivariana, Facultad de Ingeniería Mecánica,
More informationDEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS
DEVELOPMENT OF A CONTINUUM PLASTICITY MODEL FOR THE COMMERCIAL FINITE ELEMENT CODE ABAQUS Mohsen Safaei, Wim De Waele Ghent University, Laboratory Soete, Belgium Abstract The present work relates to the
More informationTHREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT
THREE DIMENSIONAL STRESS ANALYSIS OF THE T BOLT JOINT Víctor Martínez 1, Alfredo Güemes 2, Norbert Blanco 1, Josep Costa 1 1 Escola Politècnica Superior. Universitat de Girona. Girona, Spain (17071) 2
More informationDiscrete ply modelling of open hole tensile tests
Discrete ply modelling of open hole tensile tests Victor Achard, Christophe Bouvet, Bruno Castanié, Clément Chirol To cite this version: Victor Achard, Christophe Bouvet, Bruno Castanié, Clément Chirol.
More informationVIRTUAL TESTING OF ADVANCED POLYMER COMPOSITE MATERIALS. Ana Andreia Pinheiro Durão Branco. Master s Thesis Advisor: Prof. Dr. Pedro Ponces Camanho
VIRTUAL TESTING OF ADVANCED POLYMER COMPOSITE MATERIALS Ana Andreia Pinheiro Durão Branco Master s Thesis Advisor: Prof. Dr. Pedro Ponces Camanho Mestrado Integrado em Engenharia Mecânica July 17, 2015
More informationAn investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading
An investigation of the mechanical behaviour of carbon epoxy cross ply cruciform specimens under biaxial loading A. Makris, C. Ramault, D. Van Hemelrijck Department of Mechanics of Materials and Constructions,
More informationCHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS
Oral Reference Number: ICF100942OR CHARACTERIZATION, ANALYSIS AND PREDICTION OF DELAMINATION IN COMPOSITES USING FRACTURE MECHANICS T. Kevin O Brien U.S. Army Research Laboratory Vehicle Technology Directorate
More informationCalculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites
Copyright c 2007 ICCES ICCES, vol.1, no.2, pp.6167, 2007 Calculation of Energy Release Rate in Mode I Delamination of Angle Ply Laminated Composites K. Gordnian 1, H. Hadavinia 1, G. Simpson 1 and A.
More informationModeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites
Modeling and Simulations of Aircraft Structures Stiffness, Damage, and Failure Prediction for Laminated Composites H.E.Pettermann 1, C.Schuecker 1, D.H.Pahr 2, F.G.Rammerstorfer 2 1 Austrian Aeronautics
More informationFracture Mechanics of Composites with Residual Thermal Stresses
J. A. Nairn Material Science & Engineering, University of Utah, Salt Lake City, Utah 84 Fracture Mechanics of Composites with Residual Thermal Stresses The problem of calculating the energy release rate
More informationFiniteElement Analysis of Stress Concentration in ASTM D 638 Tension Specimens
Monika G. Garrell, 1 Albert J. Shih, 2 Edgar LaraCurzio, 3 and Ronald O. Scattergood 4 Journal of Testing and Evaluation, Vol. 31, No. 1 Paper ID JTE11402_311 Available online at: www.astm.org FiniteElement
More informationMultiscale modeling of failure in ABS materials
Institute of Mechanics Multiscale modeling of failure in ABS materials Martin Helbig, Thomas Seelig 15. International Conference on Deformation, Yield and Fracture of Polymers Kerkrade, April 2012 Institute
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationModelindependent approaches for the XFEM in fracture mechanics
Modelindependent approaches for the XFEM in fracture mechanics Safdar Abbas 1 Alaskar Alizada 2 and ThomasPeter Fries 2 1 Aachen Institute for Computational Engineering Science (AICES), RWTH Aachen University,
More informationCohesive band model: a triaxialitydependent cohesive model for damage to crack transition in a nonlocal implicit discontinuous Galerkin framework
University of Liège Aerospace & Mechanical Engineering Cohesive band model: a triaxialitydependent cohesive model for damage to crack transition in a nonlocal implicit discontinuous Galerkin framework
More informationCRACK GROWTH MODELLING: ENRICHED CONTINUUM VS. DISCRETE MODELS
CRACK GROWTH MODELLING: ENRICHED CONTINUUM VS. DISCRETE MODELS Vinh Phu Nguyen 1,*, Giang Dinh Nguyen 1, Daniel DiasdaCosta 2, Luming Shen 2, Chi Thanh Nguyen 1 1 School of Civil, Environmental & Mining
More informationID1160 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING
ID116 REALTIME DETECTION AND EXPLICIT FINITE ELEMENT SIMULATION OF DELAMINATION IN COMPOSITE LAMINATES UNDER IMPACT LOADING K. Minnaar and M. Zhou = School of Mechanical Engineering Georgia Institute
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationNonlinear analysis in ADINA Structures
Nonlinear analysis in ADINA Structures Theodore Sussman, Ph.D. ADINA R&D, Inc, 2016 1 Topics presented Types of nonlinearities Materially nonlinear only Geometrically nonlinear analysis Deformationdependent
More informationENGN 2290: Plasticity Computational plasticity in Abaqus
ENGN 229: Plasticity Computational plasticity in Abaqus The purpose of these exercises is to build a familiarity with using usermaterial subroutines (UMATs) in Abaqus/Standard. Abaqus/Standard is a finiteelement
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationInterlaminar fracture characterization in composite materials by using acoustic emission
5th International Symposium on NDT in Aerospace, 1315th November 2013, Singapore Interlaminar fracture characterization in composite materials by using acoustic emission Ian SILVERSIDES 1, Ahmed MASLOUHI
More informationMODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD
MODELING OF ELASTOPLASTIC MATERIALS IN FINITE ELEMENT METHOD Andrzej Skrzat, Rzeszow University of Technology, Powst. Warszawy 8, Rzeszow, Poland Abstract: Userdefined material models which can be used
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More information*MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials
14 th International LSDYNA Users Conference Session: Constitutive Modeling *MAT_PAPER and *MAT_COHESIVE_PAPER: Two New Models for Paperboard Materials Jesper Karlsson 1, Mikael Schill 1, Johan Tryding
More informationMultiscale digital image correlation of strain localization
Multiscale digital image correlation of strain localization J. Marty a, J. Réthoré a, A. Combescure a a. Laboratoire de Mécanique des Contacts et des Strcutures, INSA Lyon / UMR CNRS 5259 2 Avenue des
More informationChapter 3: Stress and Equilibrium of Deformable Bodies
Ch3StressEquilibrium Page 1 Chapter 3: Stress and Equilibrium of Deformable Bodies When structures / deformable bodies are acted upon by loads, they build up internal forces (stresses) within them to
More informationEXPERIMENTAL CHARACTERISATION AND MODELLING OF NON LINEAR STRESSSTRAIN BEHAVIOUR AND STRAIN RATE EFFECTS FOR UNIDIRECTIONAL CARBONEPOXY
EXPERIMENTAL CHARACTERISATION AND MODELLING OF NON LINEAR STRESSSTRAIN BEHAVIOUR AND STRAIN RATE EFFECTS FOR UNIDIRECTIONAL CARBONEPOXY H. Koerber a*, M. Vogler b, P. Kuhn a, P.P. Camanho c a Institute
More informationAPPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN
28 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES APPLICATION OF A SCALAR STRAINBASED DAMAGE ONSET THEORY TO THE FAILURE OF A COMPLEX COMPOSITE SPECIMEN Tuyen Tran*, Dan Simkins**, Shen Hin Lim*,
More informationMESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP
16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MESH MODELING OF ANGLEPLY LAMINATED COMPOSITE PLATES FOR DNS AND IPSAP Wanil Byun*, Seung Jo Kim*, Joris Wismans** *Seoul National University, Republic
More informationDirect Comparison of Anisotropic Damage Mechanics to Fracture Mechanics of Explicit Cracks
Direct Comparison of Anisotropic Damage Mechanics to Fracture Mechanics of Explicit Cracks John A. Nairn Wood Science and Engineering, Oregon State University, Corvallis, OR 97330, USA Tel: +15417374265
More information14. LSDYNA Forum 2016
14. LSDYNA Forum 2016 A Novel Approach to Model Laminated Glass R. Böhm, A. Haufe, A. Erhart DYNAmore GmbH Stuttgart 1 Content Introduction and Motivation Common approach to model laminated glass New
More informationLAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS
XXII. LAMINATION THEORY FOR THE STRENGTH OF FIBER COMPOSITE MATERIALS Introduction The lamination theory for the elastic stiffness of fiber composite materials is the backbone of the entire field, it holds
More informationElastic parameters prediction under dynamic loading based on the. unit cell of composites considering end constraint effect
Elastic parameters prediction under dynamic loading based on the unit cell of composites considering end constraint effect Wang Meng 1,, Fei Qingguo 1,, Zhang Peiwei 1, (1. Institute of Aerospace Machinery
More informationTensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites
Tensile Stress Acoustic Constants of Unidirectional Graphite/Epoxy Composites Journal of Reinforced Plastics and Composites, Vol. 9 (March, 1990) pp. 127133 W. H. PROSSER NASA Langley Research Center
More informationA Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials
Dublin, October 2010 A Constitutive Framework for the Numerical Analysis of Organic Soils and Directionally Dependent Materials FracMan Technology Group Dr Mark Cottrell Presentation Outline Some Physical
More informationSANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS
SANDWICH COMPOSITE BEAMS for STRUCTURAL APPLICATIONS de Aguiar, José M., josemaguiar@gmail.com Faculdade de Tecnologia de São Paulo, FATECSP Centro Estadual de Educação Tecnológica Paula Souza. CEETEPS
More informationMixedMode Decohesion Finite Elements for the Simulation of Delamination in Composite Materials
NASA/TM2002211737 MixedMode Decohesion Finite Elements for the Simulation of Delamination in Composite Materials Pedro P. Camanho University of Porto, Porto, Portugal Carlos G. Dávila Langley Research
More informationStatic and Time Dependent Failure of Fibre Reinforced Elastomeric Components. Salim Mirza Element Materials Technology Hitchin, UK
Static and Time Dependent Failure of Fibre Reinforced Elastomeric Components Salim Mirza Element Materials Technology Hitchin, UK Introduction Fibre reinforced elastomers are used in many applications,
More informationApplication of fracture mechanicsbased methodologies for failure predictions in composite structures
Application of fracture mechanicsbased methodologies for failure predictions in composite structures Zoltan Mikulik a, B. Gangadhara Prusty a, Rodney S. Thomson b, Donald W. Kelly a,* a School of Mechanical
More informationANSYS Mechanical Basic Structural Nonlinearities
Lecture 4 Rate Independent Plasticity ANSYS Mechanical Basic Structural Nonlinearities 1 Chapter Overview The following will be covered in this Chapter: A. Background Elasticity/Plasticity B. Yield Criteria
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationA Unified Model for Predicting the Open Hole Tensile and Compressive Strengths of Composite Laminates for Aerospace Applications
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationMaterials and Structures. Indian Institute of Technology Kanpur
Introduction to Composite Materials and Structures Nachiketa Tiwari Indian Institute of Technology Kanpur Lecture 16 Behavior of Unidirectional Composites Lecture Overview Mt Material ilaxes in unidirectional
More informationNonlinear Analysis of Reinforced Concrete Shells Subjected to Impact Loads
Transactions of the 7 th International Conference on Structural Mechanics in Reactor Technology (SMiRT 7) Prague, Czech Republic, August 7, 00 Paper # J0 Nonlinear Analysis of Reinforced Concrete Shells
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationDELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS
DELAMINATION CONTROL IN COMPOSITE BEAMS USING PIEZOELECTRIC ACTUATORS L Iannucci 1, M S I Shaik Dawood 1,2,3, E Greenhalgh 1 and A K Ariffin 3 1 Aeronautics Department, Imperial College London, South Kensington
More informationFailure Mode Predictions in the Compressive Response of Laminated Composites
Structures, Structural Dynamics, and Materials and Colocated Conferences April 811, 2013, Boston, Massachusetts 54th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics, and Materials Conference AIAA
More informationMechanics of Materials and Structures
Journal of Mechanics of Materials and Structures A CRITICAL ANALYSIS OF INTERFACE CONSTITUTIVE MODELS FOR THE SIMULATION OF DELAMINATION IN COMPOSITES AND FAILURE OF ADHESIVE BONDS Anton Matzenmiller,
More informationPRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses
OPTIMAT BLADES Page 1 of 24 PRELIMINARY PREDICTION OF SPECIMEN PROPERTIES CLT and 1 st order FEM analyses first issue Peter Joosse CHANGE RECORD Issue/revision date pages Summary of changes draft 241002
More informationStress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole
Stress and Displacement Analysis of a Rectangular Plate with Central Elliptical Hole Dheeraj Gunwant, J. P. Singh mailto.dheerajgunwant@gmail.com, jitenderpal2007@gmail.com, AIT, Rampur Abstract A static
More informationNumerical Characterization of Concrete Heterogeneity
Vol. Materials 5, No. Research, 3, 2002Vol. 5, No. 3, Statistical 309314, 2002. Characterization of the Concrete Numerical Modeling of Size Effect In Heterogeneity 2002 309 Numerical Characterization
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationA synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks
Article A synergistic damage mechanics approach to mechanical response of composite laminates with ply cracks JOURNAL OF COMPOSITE MATERIALS Journal of Composite Materials 0(0) 7! The Author(s) 0 Reprints
More informationMECHANICS OF MATERIALS. EQUATIONS AND THEOREMS
1 MECHANICS OF MATERIALS. EQUATIONS AND THEOREMS Version 20110114 Stress tensor Definition of traction vector (1) Cauchy theorem (2) Equilibrium (3) Invariants (4) (5) (6) or, written in terms of principal
More informationThe Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints
, June 30  July 2, 2010, London, U.K. The Accuracy of Characteristic Length Method on Failure Load Prediction of Composite Pinned Joints O. Aluko, and Q. Mazumder Abstract An analytical model was developed
More informationEnhancing Prediction Accuracy In Sift Theory
18 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS Enhancing Prediction Accuracy In Sift Theory J. Wang 1 *, W. K. Chiu 1 Defence Science and Technology Organisation, Fishermans Bend, Australia, Department
More informationSTRAIN ASSESSMENT USFOS
1 STRAIN ASSESSMENT IN USFOS 2 CONTENTS: 1 Introduction...3 2 Revised strain calculation model...3 3 Strain predictions for various characteristic cases...4 3.1 Beam with concentrated load at mid span...
More informationSIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO MULTIPLE LOADING WITH MEMBRANEFLEXION COUPLING EFFECTS
VOL. 5, NO. 4, APRIL 010 ISSN 18196608 006010 Asian Research Publishing Network (ARPN). All rights reserved. SIMULATION OF PROGRESSIVE FAILURE PREDICTION OF FILAMENT WOUND COMPOSITE TUBES SUBJECTED TO
More informationAnálisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas
San Miguel de Tucuman, Argentina September 14 th, 2011 Seminary on Análisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas Antonio Caggiano 1, Guillermo Etse 2, Enzo
More informationAnisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA
Anisotropic modeling of short fibers reinforced thermoplastics materials with LSDYNA Alexandre Hatt 1 1 Faurecia Automotive Seating, Simplified Limited Liability Company 1 Abstract / Summary Polymer thermoplastics
More informationModeling of Debonding and Crack Propagation in Fibrous Composites Using a Discontinuous Galerkin Approach
University of Tennessee, Knoxville Trace: Tennessee Research and Creative Exchange Masters Theses Graduate School 52015 Modeling of Debonding and Crack Propagation in Fibrous Composites Using a Discontinuous
More informationDETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1
PERIODICA POLYTECHNICA SER. CIV. ENG. VOL. 46, NO. 1, PP. 125 148 (2002) DETERMINING THE STRESS PATTERN IN THE HH RAILROAD TIES DUE TO DYNAMIC LOADS 1 Nándor LIEGNER Department of Highway and Railway Engineering
More informationADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF COMPOSITES
NAFEMS WORLD CONGRESS 13, SALZBURG, AUSTRIA ADVANCES IN THE PROGRESSIVE DAMAGE ANALYSIS OF M. Bruyneel, J.P. Delsemme, P. Jetteur (LMS Samtech, Belgium); A.C. Goupil (ISMANS, France). Dr. Ir. M. Bruyneel,
More information16 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS
6 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS FRACTURE INTERFACE ELEMENTS FOR STATIC AND FATIUE ANALYSIS erald E. Mabson*, Lyle R. Deobald*, Bernhard Dopker*, D.M. Hoyt**, Jeffrey S. Baylor**, Douglas
More informationBasics of Finite Element Analysis. Strength of Materials, Solid Mechanics
Basics of Finite Element Analysis Strength of Materials, Solid Mechanics 1 Outline of Presentation Basic concepts in mathematics Analogies and applications Approximations to Actual Applications Improvisation
More informationMULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS
MULTISCALE AND MULTILEVEL ANALYSIS OF COMPOSITE STRUCTURES WITH BOLTED JOINTS F.X. Irisarri, J.F. Maire* and N. Carrere ONERA, 9 av. de la Division Leclerc, 930 Châtillon, France francoisxavier.irisarri@onera.fr,
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2017 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationfive Mechanics of Materials 1 ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture
ARCHITECTURAL STRUCTURES: FORM, BEHAVIOR, AND DESIGN DR. ANNE NICHOLS SUMMER 2014 lecture five mechanics www.carttalk.com of materials Mechanics of Materials 1 Mechanics of Materials MECHANICS MATERIALS
More informationDebonding process in composites using BEM
Boundary Elements XXVII 331 Debonding process in composites using BEM P. Prochazka & M. Valek Czech Technical University, Prague, Czech Republic Abstract The paper deals with the debonding fibermatrix
More information